#------------------------------------------------------------------------------
#$Date: 2020-02-04 22:10:48 +0200 (Tue, 04 Feb 2020) $
#$Revision: 247622 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/12/56/7125641.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7125641
loop_
_publ_author_name
'Zhang, Shan'
'Lu, Ying'
'Sun, Xiu-Wei'
'Li, Zhuo'
'Dang, Tian-Yi'
'Zhang, Zhong'
'Tian, Hong-Rui'
'Liu, Shu-Xia'
_publ_section_title
;
 Purely inorganic frameworks based on polyoxometalate clusters with
 abundant phosphate groups: single-crystal to single-crystal structural
 transformation and remarkable proton conduction.
;
_journal_issue                   3
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              391
_journal_page_last               394
_journal_paper_doi               10.1039/c9cc08696j
_journal_volume                  56
_journal_year                    2020
_chemical_formula_moiety         '0.5(Fe80 Mo192 Na64 O1156 P136), 54(O)'
_chemical_formula_sum            'Fe40 Mo96 Na32 O632 P68'
_chemical_formula_weight         24397.88
_space_group_crystal_system      tetragonal
_space_group_IT_number           142
_space_group_name_Hall           '-I 4bd 2c'
_space_group_name_H-M_alt        'I 41/a c d :2'
_atom_sites_solution_primary     iterative
_audit_creation_date             2019-03-27
_audit_creation_method
;
Olex2 1.2-beta
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2019-09-25 deposited with the CCDC.	2019-11-27 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   27.3329(12)
_cell_length_b                   27.3329(12)
_cell_length_c                   37.8621(14)
_cell_measurement_reflns_used    9885
_cell_measurement_temperature    100
_cell_measurement_theta_max      26.01
_cell_measurement_theta_min      2.59
_cell_volume                     28286(2)
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_diffrn_ambient_temperature      100.0
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0398
_diffrn_reflns_av_unetI/netI     0.0207
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -33
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       45
_diffrn_reflns_limit_l_min       -44
_diffrn_reflns_number            73586
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.065
_diffrn_reflns_theta_min         2.590
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.392
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.865
_exptl_crystal_description       block
_exptl_crystal_F_000             23000
_refine_diff_density_max         1.360
_refine_diff_density_min         -1.044
_refine_diff_density_rms         0.170
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     546
_refine_ls_number_reflns         6960
_refine_ls_number_restraints     72
_refine_ls_restrained_S_all      1.058
_refine_ls_R_factor_all          0.0420
_refine_ls_R_factor_gt           0.0317
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0490P)²+461.1291P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0897
_refine_ls_wR_factor_ref         0.0962
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5905
_reflns_number_total             6960
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c9cc08696j2.cif
_cod_data_source_block           2
_cod_depositor_comments
'Adding full bibliography for 7125640--7125641.cif.'
_cod_original_cell_volume        28286(3)
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_database_code               7125641
_shelx_shelxl_version_number     2017/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O10W) \\sim Ueq, Uanis(O12W) \\sim Ueq, Uanis(O9W) \\sim Ueq, Uanis(O8W)
\\sim Ueq, Uanis(O5W) \\sim Ueq, Uanis(O11W) \\sim Ueq: with sigma of 0.01 and
sigma for terminal atoms of 0.02
Uanis(O4W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O7W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O3WA) \\sim Ueq, Uanis(O3W) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
Uanis(O6W) \\sim Ueq, Uanis(O13W) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
2. Others
 Fixed Sof: O3W(0.5) O8W(0.5) O9W(0.5) O11W(0.5) O12W(0.25) O5W(0.5) O10W(0.5)
 O4W(0.125) O3WA(0.5) O7W(0.125) O13W(0.25) O6W(0.25)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-y+1/4, x+3/4, z+1/4'
'y+1/4, -x+1/4, z+3/4'
'-x+1/2, y, -z'
'x, -y, -z+1/2'
'y+1/4, x+3/4, -z+3/4'
'-y+1/4, -x+1/4, -z+1/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-y+3/4, x+5/4, z+3/4'
'y+3/4, -x+3/4, z+5/4'
'-x+1, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1'
'y+3/4, x+5/4, -z+5/4'
'-y+3/4, -x+3/4, -z+3/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'y-1/4, -x-3/4, -z-1/4'
'-y-1/4, x-1/4, -z-3/4'
'x-1/2, -y, z'
'-x, y, z-1/2'
'-y-1/4, -x-3/4, z-3/4'
'y-1/4, x-1/4, z-1/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'y+1/4, -x-1/4, -z+1/4'
'-y+1/4, x+1/4, -z-1/4'
'x, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'-y+1/4, -x-1/4, z-1/4'
'y+1/4, x+1/4, z+1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo3 Mo 0.31973(2) 0.59680(2) 0.46697(2) 0.01249(11) Uani 1 1 d . . . . .
Mo2 Mo 0.37190(2) 0.66230(2) 0.53649(2) 0.01373(12) Uani 1 1 d . . . . .
Mo4 Mo 0.28258(2) 0.64406(2) 0.41377(2) 0.01295(11) Uani 1 1 d . . . . .
Mo1 Mo 0.37207(2) 0.75653(2) 0.53669(2) 0.01408(12) Uani 1 1 d . . . . .
Mo6 Mo 0.31912(2) 0.82029(2) 0.47172(2) 0.01690(12) Uani 1 1 d . . . . .
Mo5 Mo 0.27217(2) 0.76658(2) 0.41296(2) 0.01632(12) Uani 1 1 d . . . . .
Fe1 Fe 0.51858(3) 0.83886(3) 0.43235(2) 0.01038(16) Uani 1 1 d . . . . .
Fe2 Fe 0.250000 0.70959(4) 0.500000 0.0140(2) Uani 1 2 d S T P . .
Fe3 Fe 0.28912(3) 0.70672(3) 0.25530(2) 0.01882(19) Uani 1 1 d . . . . .
P3 P 0.37556(5) 0.70732(5) 0.45342(4) 0.0104(3) Uani 1 1 d . . . . .
P1 P 0.500000 0.750000 0.375000 0.0109(5) Uani 1 4 d S T P . .
P4 P 0.43354(5) 0.58050(5) 0.49138(4) 0.0111(3) Uani 1 1 d . . . . .
P5 P 0.31285(5) 0.70942(5) 0.34170(4) 0.0131(3) Uani 1 1 d . . . . .
P2 P 0.43425(5) 0.84193(5) 0.49202(4) 0.0135(3) Uani 1 1 d . . . . .
Na1 Na 0.41194(10) 0.81354(12) 0.41172(7) 0.0374(7) Uani 1 1 d . . . . .
Na2 Na 0.500000 0.750000 0.50841(14) 0.0459(11) Uani 1 2 d S T P . .
O22 O 0.27039(13) 0.64917(14) 0.46501(10) 0.0146(8) Uani 1 1 d . . . . .
O15 O 0.31883(14) 0.70936(14) 0.52903(10) 0.0153(8) Uani 1 1 d . . . . .
O18 O 0.27018(14) 0.76879(14) 0.46460(10) 0.0160(8) Uani 1 1 d . . . . .
O23 O 0.32067(14) 0.60791(14) 0.52159(10) 0.0157(8) Uani 1 1 d . . . . .
O16 O 0.36811(13) 0.66182(13) 0.47737(10) 0.0121(8) Uani 1 1 d . . . . .
O17 O 0.33515(14) 0.70689(13) 0.42510(10) 0.0137(8) Uani 1 1 d . . . . .
O12 O 0.36960(13) 0.75388(14) 0.47610(10) 0.0144(8) Uani 1 1 d . . . . .
O26 O 0.38443(14) 0.56018(14) 0.47719(11) 0.0169(8) Uani 1 1 d . . . . .
O13 O 0.32430(14) 0.81014(14) 0.51935(10) 0.0170(8) Uani 1 1 d . . . . .
O21 O 0.24186(14) 0.70681(14) 0.41042(10) 0.0164(8) Uani 1 1 d . . . . .
O28 O 0.46652(13) 0.53628(13) 0.50090(10) 0.0148(8) Uani 1 1 d . . . . .
O24 O 0.34217(14) 0.60525(14) 0.41849(10) 0.0151(8) Uani 1 1 d . . . . .
O4 O 0.47157(14) 0.81524(14) 0.46913(10) 0.0156(8) Uani 1 1 d . . . . .
O29 O 0.42425(14) 0.60944(14) 0.52535(10) 0.0183(8) Uani 1 1 d . . . . .
O8 O 0.38652(14) 0.85023(14) 0.47013(10) 0.0175(8) Uani 1 1 d . . . . .
O9 O 0.32769(14) 0.80862(14) 0.42106(10) 0.0177(8) Uani 1 1 d . . . . .
O11 O 0.42681(14) 0.70738(14) 0.43802(10) 0.0169(8) Uani 1 1 d . . . . .
O3 O 0.49012(14) 0.79519(14) 0.39763(10) 0.0169(8) Uani 1 1 d . . . . .
O5 O 0.57563(14) 0.79059(14) 0.53018(10) 0.0181(9) Uani 1 1 d . . . . .
O7 O 0.42415(15) 0.80925(15) 0.52416(10) 0.0198(9) Uani 1 1 d . . . . .
O34 O 0.45232(15) 0.89105(15) 0.50512(11) 0.0211(9) Uani 1 1 d . . . . .
O2 O 0.46439(14) 0.88317(14) 0.41552(11) 0.0180(8) Uani 1 1 d . . . . .
O19 O 0.29700(14) 0.75572(14) 0.36333(10) 0.0179(8) Uani 1 1 d . . . . .
O27 O 0.45826(14) 0.61031(15) 0.46321(11) 0.0203(9) Uani 1 1 d . . . . .
O1 O 0.56593(15) 0.87299(16) 0.39445(11) 0.0226(9) Uani 1 1 d . . . . .
O31 O 0.30297(15) 0.66245(14) 0.36298(10) 0.0191(9) Uani 1 1 d . . . . .
O32 O 0.28287(17) 0.70867(16) 0.30764(12) 0.0271(10) Uani 1 1 d . . . . .
O25 O 0.28524(15) 0.54583(16) 0.46617(11) 0.0237(9) Uani 1 1 d . . . . .
O20 O 0.22775(16) 0.80616(16) 0.40283(12) 0.0255(10) Uani 1 1 d . . . . .
O33 O 0.35392(15) 0.51095(15) 0.65195(11) 0.0207(9) Uani 1 1 d . . . . .
O10 O 0.28492(16) 0.87136(16) 0.47042(12) 0.0273(10) Uani 1 1 d . . . . .
O30 O 0.36874(16) 0.65038(16) 0.58015(11) 0.0249(10) Uani 1 1 d . . . . .
O14 O 0.37077(16) 0.76838(16) 0.58006(11) 0.0240(9) Uani 1 1 d . . . . .
Na3 Na 0.34122(16) 0.59122(16) 0.625000 0.0767(18) Uani 1 2 d S T P . .
O1W O 0.28267(19) 0.7068(2) 0.19739(14) 0.0426(13) Uani 1 1 d . . . . .
O2W O 0.28282(19) 0.6304(2) 0.25252(16) 0.0454(14) Uani 1 1 d . . . . .
O3W O 0.2753(10) 0.5898(9) 0.6815(7) 0.111(8) Uani 0.5 1 d . U . A 1
O8W O 0.5518(6) 0.9240(5) 0.6004(3) 0.066(4) Uani 0.5 1 d . U . . .
O9W O 0.4975(4) 0.8849(5) 0.5628(3) 0.057(3) Uani 0.5 1 d . U . . .
O11W O 0.3293(6) 0.9100(5) 0.5493(4) 0.087(5) Uani 0.5 1 d . U . . .
O12W O 0.250000 0.9617(8) 0.500000 0.104(8) Uani 0.5 2 d S TU P . .
O5W O 0.3734(7) 0.5003(7) 0.4074(5) 0.106(6) Uani 0.5 1 d . U . . .
O10W O 0.4349(9) 0.8775(8) 0.5933(6) 0.140(8) Uani 0.5 1 d . U . . .
O4W O 0.500000 0.750000 0.5780(8) 0.054(8) Uani 0.25 2 d S TU P . .
O3WA O 0.2917(8) 0.6159(10) 0.6721(6) 0.101(7) Uani 0.5 1 d . U . A 2
O7W O 0.4498(12) 0.6998(12) 0.625000 0.097(13) Uani 0.25 2 d S TU P . .
O13W O 0.3342(17) 0.5364(17) 0.3567(11) 0.133(14) Uani 0.25 1 d . U . . .
O6W O 0.2480(16) 0.4696(15) 0.4301(12) 0.122(13) Uani 0.25 1 d . U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O22 Mo3 Mo4 48.83(11) . .
O22 Mo3 O23 86.57(15) . .
O22 Mo3 O16 80.49(15) . .
O22 Mo3 O26 160.88(16) . .
O23 Mo3 Mo4 134.37(11) . .
O23 Mo3 O16 72.83(14) . .
O16 Mo3 Mo4 88.43(9) . .
O26 Mo3 Mo4 135.99(11) . .
O26 Mo3 O23 82.80(15) . .
O26 Mo3 O16 81.20(14) . .
O24 Mo3 Mo4 48.26(11) . .
O24 Mo3 O22 95.39(15) . .
O24 Mo3 O23 155.59(15) . .
O24 Mo3 O16 83.47(15) . .
O24 Mo3 O26 87.96(16) . .
O25 Mo3 Mo4 100.29(15) . .
O25 Mo3 O22 102.57(19) . .
O25 Mo3 O23 98.34(18) . .
O25 Mo3 O16 170.60(17) . .
O25 Mo3 O26 94.69(18) . .
O25 Mo3 O24 104.92(19) . .
O15 Mo2 Mo1 49.09(11) . .
O15 Mo2 O23 86.16(15) . .
O15 Mo2 O16 79.96(15) . .
O15 Mo2 O29 159.65(16) . .
O23 Mo2 Mo1 134.72(11) . .
O23 Mo2 O16 72.50(14) . .
O16 Mo2 Mo1 90.50(9) . .
O29 Mo2 Mo1 134.02(12) . .
O29 Mo2 O23 85.01(15) . .
O29 Mo2 O16 79.91(14) . .
O5 Mo2 Mo1 48.39(11) 10_564 .
O5 Mo2 O15 95.37(16) 10_564 .
O5 Mo2 O23 156.99(16) 10_564 .
O5 Mo2 O16 85.13(15) 10_564 .
O5 Mo2 O29 85.84(16) 10_564 .
O30 Mo2 Mo1 100.97(15) . .
O30 Mo2 O15 103.31(19) . .
O30 Mo2 O23 95.27(19) . .
O30 Mo2 O16 167.24(18) . .
O30 Mo2 O29 95.74(18) . .
O30 Mo2 O5 106.6(2) . 10_564
O22 Mo4 Mo3 48.65(11) . .
O22 Mo4 O17 82.42(15) . .
O22 Mo4 O21 84.82(15) . .
O22 Mo4 O31 160.76(16) . .
O17 Mo4 Mo3 88.99(9) . .
O21 Mo4 Mo3 132.55(11) . .
O21 Mo4 O17 73.94(14) . .
O21 Mo4 O31 83.40(16) . .
O24 Mo4 Mo3 48.17(11) . .
O24 Mo4 O22 95.13(15) . .
O24 Mo4 O17 82.31(14) . .
O24 Mo4 O21 156.07(16) . .
O24 Mo4 O31 89.56(16) . .
O31 Mo4 Mo3 137.52(12) . .
O31 Mo4 O17 79.73(15) . .
O33 Mo4 Mo3 99.13(14) 11_544 .
O33 Mo4 O22 100.87(18) 11_544 .
O33 Mo4 O17 171.44(17) 11_544 .
O33 Mo4 O21 98.36(18) 11_544 .
O33 Mo4 O24 105.11(18) 11_544 .
O33 Mo4 O31 95.86(18) 11_544 .
O15 Mo1 Mo2 48.88(11) . .
O15 Mo1 O12 79.06(15) . .
O15 Mo1 O13 87.16(16) . .
O15 Mo1 O7 158.01(16) . .
O12 Mo1 Mo2 88.02(10) . .
O13 Mo1 Mo2 134.91(11) . .
O13 Mo1 O12 71.76(14) . .
O13 Mo1 O7 82.47(16) . .
O5 Mo1 Mo2 48.47(12) 10_564 .
O5 Mo1 O15 95.24(16) 10_564 .
O5 Mo1 O12 82.75(15) 10_564 .
O5 Mo1 O13 153.48(16) 10_564 .
O5 Mo1 O7 85.79(17) 10_564 .
O7 Mo1 Mo2 133.89(12) . .
O7 Mo1 O12 79.29(14) . .
O14 Mo1 Mo2 101.31(15) . .
O14 Mo1 O15 104.82(19) . .
O14 Mo1 O12 170.22(18) . .
O14 Mo1 O13 99.25(19) . .
O14 Mo1 O5 105.58(19) . 10_564
O14 Mo1 O7 95.99(19) . .
O18 Mo6 Mo5 40.92(11) . .
O18 Mo6 O12 81.47(15) . .
O18 Mo6 O8 155.58(16) . .
O12 Mo6 Mo5 85.54(10) . .
O13 Mo6 Mo5 134.38(13) . .
O13 Mo6 O18 94.56(17) . .
O13 Mo6 O12 76.21(15) . .
O13 Mo6 O8 91.16(17) . .
O13 Mo6 O9 158.61(17) . .
O8 Mo6 Mo5 125.11(11) . .
O8 Mo6 O12 76.88(15) . .
O9 Mo6 Mo5 40.05(11) . .
O9 Mo6 O18 80.21(16) . .
O9 Mo6 O12 82.50(15) . .
O9 Mo6 O8 85.85(16) . .
O10 Mo6 Mo5 98.56(16) . .
O10 Mo6 O18 102.3(2) . .
O10 Mo6 O12 175.77(19) . .
O10 Mo6 O13 101.4(2) . .
O10 Mo6 O8 99.8(2) . .
O10 Mo6 O9 100.0(2) . .
O18 Mo5 Mo6 41.00(11) . .
O18 Mo5 O17 81.40(15) . .
O18 Mo5 O19 160.63(16) . .
O17 Mo5 Mo6 83.28(9) . .
O21 Mo5 Mo6 132.63(12) . .
O21 Mo5 O18 93.86(17) . .
O21 Mo5 O17 74.36(15) . .
O21 Mo5 O9 153.46(17) . .
O21 Mo5 O19 88.40(17) . .
O9 Mo5 Mo6 40.82(12) . .
O9 Mo5 O18 81.05(16) . .
O9 Mo5 O17 79.13(15) . .
O9 Mo5 O19 88.35(17) . .
O19 Mo5 Mo6 128.82(12) . .
O19 Mo5 O17 80.70(14) . .
O20 Mo5 Mo6 99.58(16) . .
O20 Mo5 O18 100.90(19) . .
O20 Mo5 O17 177.13(19) . .
O20 Mo5 O21 103.7(2) . .
O20 Mo5 O9 102.9(2) . .
O20 Mo5 O19 97.23(19) . .
O4 Fe1 O2 86.68(16) . .
O4 Fe1 O1 173.02(17) . .
O11 Fe1 O4 101.77(17) 10_564 .
O11 Fe1 O2 167.80(17) 10_564 .
O11 Fe1 O1 83.95(17) 10_564 .
O3 Fe1 O4 90.89(16) . .
O3 Fe1 O11 89.01(16) . 10_564
O3 Fe1 O2 82.00(17) . .
O3 Fe1 O1 93.22(17) . .
O2 Fe1 O1 88.31(16) . .
O27 Fe1 O4 91.24(17) 10_564 .
O27 Fe1 O11 98.52(16) 10_564 10_564
O27 Fe1 O3 171.58(18) 10_564 .
O27 Fe1 O2 89.99(17) 10_564 .
O27 Fe1 O1 83.90(18) 10_564 .
O22 Fe2 O22 82.1(2) 5_556 .
O15 Fe2 O22 84.97(14) . 5_556
O15 Fe2 O22 94.78(14) . .
O15 Fe2 O22 94.78(14) 5_556 5_556
O15 Fe2 O22 84.97(14) 5_556 .
O15 Fe2 O15 179.7(2) . 5_556
O18 Fe2 O22 179.13(14) . 5_556
O18 Fe2 O22 97.12(14) 5_556 5_556
O18 Fe2 O22 97.12(14) . .
O18 Fe2 O22 179.13(14) 5_556 .
O18 Fe2 O15 95.40(14) 5_556 5_556
O18 Fe2 O15 84.85(14) . 5_556
O18 Fe2 O15 84.84(14) 5_556 .
O18 Fe2 O15 95.40(14) . .
O18 Fe2 O18 83.7(2) . 5_556
O28 Fe3 O28 80.05(16) 11_544 19_576
O28 Fe3 O1W 83.42(19) 19_576 .
O28 Fe3 O1W 80.85(18) 11_544 .
O28 Fe3 O2W 92.45(18) 11_544 .
O34 Fe3 O28 94.29(16) 28_656 19_576
O34 Fe3 O28 163.34(17) 28_656 11_544
O34 Fe3 O32 106.65(18) 28_656 .
O34 Fe3 O1W 82.95(19) 28_656 .
O34 Fe3 O2W 90.51(19) 28_656 .
O32 Fe3 O28 89.50(17) . 11_544
O32 Fe3 O28 94.64(17) . 19_576
O32 Fe3 O1W 170.34(19) . .
O32 Fe3 O2W 94.0(2) . .
O2W Fe3 O28 168.5(2) . 19_576
O2W Fe3 O1W 86.8(2) . .
O17 P3 O16 107.9(2) . .
O17 P3 O12 108.5(2) . .
O12 P3 O16 108.7(2) . .
O11 P3 O16 110.3(2) . .
O11 P3 O17 113.3(2) . .
O11 P3 O12 108.1(2) . .
O3 P1 O3 108.36(15) 28_656 10_564
O3 P1 O3 108.35(15) . 19_576
O3 P1 O3 111.7(3) 28_656 19_576
O3 P1 O3 108.35(15) . 28_656
O3 P1 O3 108.36(15) 19_576 10_564
O3 P1 O3 111.7(3) . 10_564
O26 P4 O28 107.7(2) . .
O29 P4 O26 109.4(2) . .
O29 P4 O28 107.7(2) . .
O27 P4 O26 109.8(2) . .
O27 P4 O28 109.1(2) . .
O27 P4 O29 113.0(2) . .
O2 P5 O19 107.0(2) 28_656 .
O2 P5 O31 110.0(2) 28_656 .
O2 P5 O32 111.9(3) 28_656 .
O31 P5 O19 110.6(2) . .
O32 P5 O19 107.7(2) . .
O32 P5 O31 109.7(2) . .
O4 P2 O8 109.1(2) . .
O4 P2 O7 107.0(2) . .
O7 P2 O8 110.8(2) . .
O34 P2 O4 113.1(2) . .
O34 P2 O8 108.5(2) . .
O34 P2 O7 108.4(2) . .
O8 Na1 O4 57.16(13) . .
O9 Na1 O4 118.15(17) . .
O9 Na1 O8 67.60(15) . .
O9 Na1 O2 129.01(19) . .
O3 Na1 O4 67.98(14) . .
O3 Na1 O8 123.71(17) . .
O3 Na1 O9 163.0(2) . .
O3 Na1 O2 67.86(15) . .
O3 Na1 O1 100.26(17) . 28_656
O2 Na1 O4 65.03(14) . .
O2 Na1 O8 78.22(16) . .
O1 Na1 O4 167.04(18) 28_656 .
O1 Na1 O8 132.44(18) 28_656 .
O1 Na1 O9 74.68(16) 28_656 .
O1 Na1 O2 106.17(19) 28_656 .
P2 Na2 Mo1 58.26(3) 10_564 10_564
Na2 Na2 Mo1 0(4) 10_564 10_564
Na2 Na2 P2 0(10) 10_564 10_564
Na2 Na2 O4 0(10) 10_564 10_564
Na2 Na2 O4 0(10) 10_564 .
Na2 Na2 O5 0(10) 10_564 10_564
Na2 Na2 O5 0(10) 10_564 .
Na2 Na2 O7 0(10) 10_564 .
Na2 Na2 O7 0(10) 10_564 10_564
Na2 Na2 O4W 0(10) 10_564 .
O4 Na2 Mo1 121.08(10) . 10_564
O4 Na2 Mo1 80.74(9) 10_564 10_564
O4 Na2 P2 28.19(9) 10_564 10_564
O4 Na2 P2 129.9(2) . 10_564
O4 Na2 O4 105.2(3) 10_564 .
O4 Na2 O5 98.06(13) . .
O4 Na2 O5 98.06(13) 10_564 10_564
O4 Na2 O5 105.22(14) . 10_564
O4 Na2 O5 105.22(14) 10_564 .
O4 Na2 O7 144.62(19) . 10_564
O4 Na2 O7 56.85(12) . .
O4 Na2 O7 56.85(12) 10_564 10_564
O4 Na2 O7 144.62(19) 10_564 .
O4 Na2 O4W 127.40(13) . .
O4 Na2 O4W 127.40(13) 10_564 .
O5 Na2 Mo1 132.47(17) 10_564 10_564
O5 Na2 Mo1 29.64(9) . 10_564
O5 Na2 P2 86.96(9) . 10_564
O5 Na2 P2 100.59(9) 10_564 10_564
O5 Na2 O5 141.3(3) . 10_564
O5 Na2 O7 107.33(15) 10_564 10_564
O5 Na2 O7 63.61(13) . 10_564
O5 Na2 O7 107.33(15) . .
O5 Na2 O7 63.61(13) 10_564 .
O5 Na2 O4W 70.64(14) . .
O5 Na2 O4W 70.64(14) 10_564 .
O7 Na2 Mo1 34.11(9) 10_564 10_564
O7 Na2 Mo1 134.32(15) . 10_564
O7 Na2 P2 29.13(9) 10_564 10_564
O7 Na2 P2 163.87(9) . 10_564
O7 Na2 O7 154.5(3) 10_564 .
O4W Na2 Mo1 73.00(8) . 10_564
O4W Na2 P2 101.36(10) . 10_564
O4W Na2 O7 77.23(14) . .
O4W Na2 O7 77.23(14) . 10_564
Mo3 O22 Mo4 82.52(15) . .
Mo3 O22 Fe2 134.44(19) . .
Mo4 O22 Fe2 133.74(19) . .
Mo2 O15 Mo1 82.03(15) . .
Mo2 O15 Fe2 135.5(2) . .
Mo1 O15 Fe2 135.37(19) . .
Mo6 O18 Fe2 128.56(19) . .
Mo5 O18 Mo6 98.08(17) . .
Mo5 O18 Fe2 126.90(19) . .
Mo3 O23 Mo2 111.94(17) . .
Mo2 O16 Mo3 101.92(14) . .
P3 O16 Mo3 127.4(2) . .
P3 O16 Mo2 124.9(2) . .
Mo4 O17 Mo5 91.37(13) . .
P3 O17 Mo4 126.1(2) . .
P3 O17 Mo5 129.7(2) . .
Mo6 O12 Mo1 93.72(14) . .
P3 O12 Mo1 125.4(2) . .
P3 O12 Mo6 132.7(2) . .
P4 O26 Mo3 129.2(2) . .
Mo6 O13 Mo1 117.95(19) . .
Mo5 O21 Mo4 119.8(2) . .
Fe3 O28 Fe3 99.95(16) 12_454 28_656
P4 O28 Fe3 135.6(2) . 12_454
P4 O28 Fe3 121.5(2) . 28_656
Mo3 O24 Mo4 83.57(14) . .
Fe1 O4 Na1 80.46(14) . .
Fe1 O4 Na2 116.99(18) . .
Fe1 O4 Na2 116.99(18) . 10_564
P2 O4 Fe1 132.1(2) . .
P2 O4 Na1 93.52(19) . .
P2 O4 Na2 102.4(2) . 10_564
P2 O4 Na2 102.4(2) . .
Na2 O4 Na1 131.59(18) . .
Na2 O4 Na1 131.59(18) 10_564 .
Na2 O4 Na2 0.00(19) 10_564 .
P4 O29 Mo2 130.1(2) . .
Mo6 O8 Na1 96.67(16) . .
P2 O8 Mo6 133.5(2) . .
P2 O8 Na1 100.2(2) . .
Mo6 O9 Na1 104.90(18) . .
Mo5 O9 Mo6 99.13(18) . .
Mo5 O9 Na1 141.9(2) . .
P3 O11 Fe1 137.9(2) . 10_564
Fe1 O3 Na1 94.75(16) . .
P1 O3 Fe1 143.9(2) . .
P1 O3 Na1 118.6(2) . .
Mo2 O5 Na2 161.9(2) 10_564 .
Mo2 O5 Na2 161.9(2) 10_564 10_564
Mo1 O5 Mo2 83.13(16) 10_564 10_564
Mo1 O5 Na2 111.01(17) 10_564 10_564
Mo1 O5 Na2 111.01(17) 10_564 .
Na2 O5 Na2 0.0(2) . 10_564
Mo1 O7 Na2 99.24(16) . .
Mo1 O7 Na2 99.24(16) . 10_564
P2 O7 Mo1 135.0(2) . .
P2 O7 Na2 92.1(2) . .
P2 O7 Na2 92.1(2) . 10_564
Na2 O7 Na2 0.0(2) 10_564 .
P2 O34 Fe3 145.1(3) . 19_576
Fe1 O2 Na1 88.93(16) . .
P5 O2 Fe1 135.4(2) 19_576 .
P5 O2 Na1 135.7(2) 19_576 .
P5 O19 Mo5 134.2(2) . .
P4 O27 Fe1 166.2(3) . 10_564
Fe1 O1 Na1 114.5(2) . 19_576
P5 O31 Mo4 137.5(2) . .
P5 O32 Fe3 142.6(3) . .
Mo4 O33 Na3 147.1(3) 12_454 .
Mo2 O30 Na3 144.9(3) . .
O33 Na3 O33 115.4(3) . 15_445
O33 Na3 O30 83.86(14) 15_445 .
O33 Na3 O30 83.86(14) . 15_445
O33 Na3 O30 146.50(15) . .
O33 Na3 O30 146.50(15) 15_445 15_445
O33 Na3 O3W 75.1(5) . 15_445
O33 Na3 O3W 75.1(5) 15_445 .
O33 Na3 O3W 76.1(5) 15_445 15_445
O33 Na3 O3W 76.1(5) . .
O30 Na3 O30 94.3(3) . 15_445
O30 Na3 O3W 84.2(5) . 15_445
O30 Na3 O3W 84.2(5) 15_445 .
O30 Na3 O3W 137.2(5) 15_445 15_445
O30 Na3 O3W 137.2(5) . .
O3W Na3 O3W 124.6(11) . 15_445
O3WA Na3 O33 76.0(5) 15_445 .
O3WA Na3 O33 91.3(7) 15_445 15_445
O3WA Na3 O33 91.3(7) . .
O3WA Na3 O33 76.0(5) . 15_445
O3WA Na3 O30 120.8(7) 15_445 15_445
O3WA Na3 O30 76.5(5) . 15_445
O3WA Na3 O30 76.5(5) 15_445 .
O3WA Na3 O30 120.8(7) . .
O3WA Na3 O3W 139.6(8) . 15_445
O3WA Na3 O3W 17.8(8) 15_445 15_445
O3WA Na3 O3WA 156.3(13) . 15_445
Na2 O4W Na2 0.0 10_564 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo3 Mo4 2.5994(7) .
Mo3 O22 1.968(4) .
Mo3 O23 2.090(4) .
Mo3 O16 2.250(4) .
Mo3 O26 2.069(4) .
Mo3 O24 1.949(4) .
Mo3 O25 1.682(4) .
Mo2 Mo1 2.5757(7) .
Mo2 O15 1.959(4) .
Mo2 O23 2.119(4) .
Mo2 O16 2.241(4) .
Mo2 O29 2.077(4) .
Mo2 O5 1.942(4) 10_564
Mo2 O30 1.687(4) .
Mo4 O22 1.974(4) .
Mo4 O17 2.280(4) .
Mo4 O21 2.049(4) .
Mo4 O24 1.952(4) .
Mo4 O31 2.064(4) .
Mo4 O33 1.679(4) 11_544
Mo1 O15 1.966(4) .
Mo1 O12 2.296(4) .
Mo1 O13 2.069(4) .
Mo1 O5 1.940(4) 10_564
Mo1 O7 2.080(4) .
Mo1 O14 1.674(4) .
Mo6 Mo5 2.9584(7) .
Mo6 O18 1.960(4) .
Mo6 O12 2.286(4) .
Mo6 O13 1.830(4) .
Mo6 O8 2.017(4) .
Mo6 O9 1.959(4) .
Mo6 O10 1.681(4) .
Mo5 O18 1.957(4) .
Mo5 O17 2.416(4) .
Mo5 O21 1.834(4) .
Mo5 O9 1.928(4) .
Mo5 O19 2.020(4) .
Mo5 O20 1.671(4) .
Fe1 O4 2.001(4) .
Fe1 O11 1.968(4) 10_564
Fe1 O3 1.939(4) .
Fe1 O2 2.017(4) .
Fe1 O27 1.922(4) 10_564
Fe1 O1 2.146(4) .
Fe2 O22 2.189(4) .
Fe2 O22 2.189(4) 5_556
Fe2 O15 2.179(4) .
Fe2 O15 2.179(4) 5_556
Fe2 O18 2.172(4) 5_556
Fe2 O18 2.172(4) .
Fe3 O28 2.085(4) 11_544
Fe3 O28 2.113(4) 19_576
Fe3 O34 1.953(4) 28_656
Fe3 O32 1.990(5) .
Fe3 O1W 2.200(5) .
Fe3 O2W 2.097(5) .
P3 O16 1.553(4) .
P3 O17 1.539(4) .
P3 O12 1.544(4) .
P3 O11 1.517(4) .
P1 O3 1.527(4) 28_656
P1 O3 1.527(4) 10_564
P1 O3 1.527(4) 19_576
P1 O3 1.527(4) .
P4 O26 1.549(4) .
P4 O28 1.550(4) .
P4 O29 1.531(4) .
P4 O27 1.503(4) .
P5 O2 1.507(4) 28_656
P5 O19 1.568(4) .
P5 O31 1.539(4) .
P5 O32 1.528(4) .
P2 O4 1.524(4) .
P2 O8 1.562(4) .
P2 O7 1.535(4) .
P2 O34 1.514(4) .
Na1 O4 2.717(5) .
Na1 O8 2.526(5) .
Na1 O9 2.333(5) .
Na1 O3 2.259(5) .
Na1 O2 2.387(5) .
Na1 O1 2.332(5) 28_656
Na2 Na2 0.000(10) 10_564
Na2 O4 2.449(5) .
Na2 O4 2.449(5) 10_564
Na2 O5 2.487(4) 10_564
Na2 O5 2.487(4) .
Na2 O7 2.698(4) .
Na2 O7 2.698(4) 10_564
Na2 O4W 2.64(3) .
O33 Na3 2.444(5) .
O30 Na3 2.462(6) .
Na3 O3W 2.80(3) 15_445
Na3 O3W 2.80(3) .
Na3 O3WA 2.34(2) 15_445
Na3 O3WA 2.34(2) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
Mo1 Mo2 O30 Na3 152.2(4) . .
Mo6 Mo5 O21 Mo4 -71.4(3) . .
Mo5 Mo6 O13 Mo1 74.7(2) . .
O15 Mo2 O30 Na3 102.0(4) . .
O18 Mo6 O13 Mo1 85.3(2) . .
O18 Mo5 O21 Mo4 -86.4(2) . .
O23 Mo2 O30 Na3 14.7(4) . .
O16 Mo2 O30 Na3 -1.5(11) . .
O16 P3 O17 Mo4 -10.3(3) . .
O16 P3 O17 Mo5 119.7(3) . .
O16 P3 O12 Mo1 16.5(3) . .
O16 P3 O12 Mo6 -123.2(3) . .
O16 P3 O11 Fe1 14.9(4) . 10_564
O17 Mo5 O21 Mo4 -6.45(19) . .
O17 P3 O16 Mo3 13.2(3) . .
O17 P3 O16 Mo2 -135.2(2) . .
O17 P3 O12 Mo1 133.6(2) . .
O17 P3 O12 Mo6 -6.1(4) . .
O17 P3 O11 Fe1 -106.1(4) . 10_564
O12 Mo6 O13 Mo1 5.29(19) . .
O12 P3 O16 Mo3 130.8(2) . .
O12 P3 O16 Mo2 -17.6(3) . .
O12 P3 O17 Mo4 -128.0(2) . .
O12 P3 O17 Mo5 2.0(3) . .
O12 P3 O11 Fe1 133.6(4) . 10_564
O26 P4 O28 Fe3 -10.0(4) . 12_454
O26 P4 O28 Fe3 146.4(2) . 28_656
O26 P4 O29 Mo2 -47.0(4) . .
O26 P4 O27 Fe1 91.4(12) . 10_564
O28 P4 O26 Mo3 169.3(3) . .
O28 P4 O29 Mo2 -163.9(3) . .
O28 P4 O27 Fe1 -150.8(12) . 10_564
O4 P2 O8 Mo6 107.8(3) . .
O4 P2 O8 Na1 -1.7(2) . .
O4 P2 O7 Mo1 -94.2(4) . .
O4 P2 O7 Na2 11.1(2) . 10_564
O4 P2 O7 Na2 11.1(2) . .
O4 P2 O34 Fe3 88.9(5) . 19_576
O29 Mo2 O30 Na3 -70.8(4) . .
O29 P4 O26 Mo3 52.5(4) . .
O29 P4 O28 Fe3 -95.7(3) . 28_656
O29 P4 O28 Fe3 107.9(3) . 12_454
O29 P4 O27 Fe1 -31.0(13) . 10_564
O8 Mo6 O13 Mo1 -70.9(2) . .
O8 P2 O4 Fe1 81.9(3) . .
O8 P2 O4 Na1 1.6(2) . .
O8 P2 O4 Na2 -132.4(2) . .
O8 P2 O4 Na2 -132.4(2) . 10_564
O8 P2 O7 Mo1 24.6(4) . .
O8 P2 O7 Na2 129.9(2) . 10_564
O8 P2 O7 Na2 129.9(2) . .
O8 P2 O34 Fe3 -32.3(5) . 19_576
O9 Mo6 O13 Mo1 10.7(6) . .
O9 Mo5 O21 Mo4 -8.7(5) . .
O11 P3 O16 Mo3 -110.9(3) . .
O11 P3 O16 Mo2 100.7(3) . .
O11 P3 O17 Mo4 112.0(3) . .
O11 P3 O17 Mo5 -118.0(3) . .
O11 P3 O12 Mo1 -103.2(3) . .
O11 P3 O12 Mo6 117.1(3) . .
O3 P1 O3 Fe1 -178.1(5) 28_656 .
O3 P1 O3 Fe1 -56.7(3) 19_576 .
O3 P1 O3 Fe1 62.6(4) 10_564 .
O3 P1 O3 Na1 148.1(3) 19_576 .
O3 P1 O3 Na1 26.71(18) 28_656 .
O3 P1 O3 Na1 -92.6(2) 10_564 .
O5 Mo2 O30 Na3 -158.2(4) 10_564 .
O7 P2 O4 Fe1 -158.2(3) . .
O7 P2 O4 Na1 121.5(2) . .
O7 P2 O4 Na2 -12.5(2) . 10_564
O7 P2 O4 Na2 -12.5(2) . .
O7 P2 O8 Mo6 -9.8(4) . .
O7 P2 O8 Na1 -119.3(2) . .
O7 P2 O34 Fe3 -152.6(4) . 19_576
O34 P2 O4 Fe1 -39.0(4) . .
O34 P2 O4 Na1 -119.3(2) . .
O34 P2 O4 Na2 106.7(2) . 10_564
O34 P2 O4 Na2 106.7(2) . .
O34 P2 O8 Mo6 -128.6(3) . .
O34 P2 O8 Na1 121.9(2) . .
O34 P2 O7 Mo1 143.6(3) . .
O34 P2 O7 Na2 -111.2(2) . .
O34 P2 O7 Na2 -111.2(2) . 10_564
O2 P5 O19 Mo5 -114.2(3) 28_656 .
O2 P5 O31 Mo4 108.7(4) 28_656 .
O2 P5 O32 Fe3 6.8(5) 28_656 .
O19 Mo5 O21 Mo4 74.3(2) . .
O19 P5 O31 Mo4 -9.3(4) . .
O19 P5 O32 Fe3 124.1(4) . .
O27 P4 O26 Mo3 -72.1(3) . .
O27 P4 O28 Fe3 27.3(3) . 28_656
O27 P4 O28 Fe3 -129.1(3) . 12_454
O27 P4 O29 Mo2 75.6(4) . .
O31 P5 O19 Mo5 5.6(4) . .
O31 P5 O32 Fe3 -115.6(4) . .
O32 P5 O19 Mo5 125.4(3) . .
O32 P5 O31 Mo4 -127.8(4) . .
O20 Mo5 O21 Mo4 171.4(2) . .
O10 Mo6 O13 Mo1 -171.1(2) . .
